Table 86. Continued. 







Exposure 

 (day) 



Depth 

 (ft) 



Corrosion 





Alloy 



Environment 



Rate 

 (mpy) 



•r b 

 Type 



Source 



Lead, tellurium 



S 



197 



2,340 



0.3 



U 



lNCO(3) 



Lead, tellurium 



W 



402 



2,370 



0.2 



u 



INCO (3) 



Lead, tellurium 



S 



402 



2,3 70 



0.3 



u 



INCO (3) 



Lead, tellurium 



W 



182 



5 



1.0 



u 



lNCO(3) 



Lead, tellurium 



W 



366 



5 



0.5 



u 



INCO (3) 



Lead-tin solder 



w 



123 



5,640 



1.2 



u 



INCO (3) 



Lead-tin solder 



s 



123 



5,640 



0.7 



u 



INCO (3) 



Lead-tin solder 



w 



403 



6,780 



1.1 



u 



INCO (3) 



Lead-tin solder 



s 



403 



6,780 



0.6 



u 



INCO (3) 



Lead-tin solder 



w 



751 



5,640 



0.3 



u 



INCO (3) 



Lead-tin solder 



s 



751 



5,640 



0.4 



u 



INCO (3) 



Lead-tin solder 



w 



1,064 



5,300 



0.3 



u 



INCO (3) 



Lead-tin solder 



s 



1,064 



5,300 



0.5 



G 



INCO (3) 



Lead-tin solder 



w 



197 



2,340 



0.5 



u 



INCO (3) 



Lead-tin solder 



s 



197 



2,340 



0.3 



u 



INCO (3) 



Lead-tin solder 



w 



402 



2,370 



0.6 



u 



INCO (3) 



Lead-tin solder 



s 



402 



2,3 70 



0.7 



u 



INCO (3) 



Lead-tin solder 



w 



182 



5 



3.7 



u 



INCO (3) 



Lead-tin solder 



w 



366 



5 



1.5 



G 



INCO (3) 



Magnesium, MIA 



w 



123 



5,640 



42.0 



s 



INCO (3) 



Magnesium, MIA 



s 



123 



5,640 



43.0 



s 



INCO (3) 



Magnesium, MIA 



w 



403 



6,780 



>20.0 



100C 



INCO (3) 



Magnesium, MIA 



s 



403 



6.780 



7.3 



S-G 



INCO (3) 



Magnesium, MIA 



vv 



751 



5,640 



>10.0 



100C 



INCO (3) 



Magnesium, MIA 



s 



751 



5,640 



>12.0 



100C 



INCO (3) 



Magnesium, MIA 



w 



1,064 



5,300 



- 



100C 



INCO (3) 



Magnesium, MIA 



s 



1,064 



5,300 



2.9 



s 



INCO (3) 



Magnesium, MIA 



vy 



197 



2,340 



- 



100C 



INCO (3) 



Magnesium, MIA 



s 



197 



2,340 



9.0 



s 



INCO (3) 



Magnesium, AZ31B 



vv 



123 



5,640 



>59.0 



100C 



INCO (3) 



Magnesium, AZ31B 



vv 



123 



5,640 



- 



P (PR) 



NADC (7) 



Magnesium, AZ31B 



s 



123 



5,640 



27.0 



s 



INCO (3) 



Magnesium, AZ31B 



w 



403 



6,780 



>20.0 



100C 



INCO (3) 



Magnesium, AZ31B 



w 



403 



6,780 



- 



N-P (PR) 



NADC (7) 



Magnesium, AZ31B 



s 



403 



6,780 



6.6 



S-G 



INCO (3) 



Magnesium, AZ31B 



w 



751 



5,640 



>10.0 



100C 



INCO (3) 



Magnesium, AZ31B 



s 



751 



5,640 



>10.0 



100C 



INCO (3) 



Magnesium, AZ31B 



vv 



1,064 



5,300 



- 



100C 



INCO (3) 



Magnesium, AZ31B 



s 



1,064 



5,300 



> 7.0 



100C 



INCO (3) 



Magnesium, AZ31B 



w 



197 



2,340 



- 



100C 



INCO (3) 



Magnesium, AZ31B 



w 



197 



2,340 



- 



EX-G 



NADC (7) 



Magnesium, AZ31B 



s 



197 



2,340 



>15.0 



50C 



INCO (3) 



Magnesium, AZ31B 



vv 



402 



2,3 70 



- 



100C 



INCO (3) 



Magnesium, AZ31B 



s 



402 



2,370 



11.0 



S 



INCO (3) 



Magnesium, AZ31B 



vv 



182 



5 



>40.0 



95C 



INCO (3) 



Magnesium, AZ31B 



vv 



366 



5 



>20.0 



100C 



INCO (3) 



248 



